| ||Format||Pages||Price|| |
|6||$44.00||  ADD TO CART|
|Hardcopy (shipping and handling)||6||$44.00||  ADD TO CART|
|Standard + Redline PDF Bundle||12||$52.80||  ADD TO CART|
This test method provides a uniform procedure for radiographic examination of weldments using industrial radiographic film. Requirements expressed in this method are intended to control the quality of the radiographic images and are not intended for controlling acceptability or quality of welds. The apparatus shall comprise of a radiation source which may be X-ray or gamma-ray source; film holders and cassettes; intensifying screens such as lead-foil, fluorescent, fluorometallic, or other metallic screens; filters which shall be used whenever the contrast reductions caused by low energy, scattered radiation, or the extent of undercut (edge burn-off) occurring on production radiographs are of significant magnitude to cause difficulty in meeting the quality level or radiographic coverage requirements stipulated by the job order or contract; masking to improve radiographic quality; IQI's or penetrameters; shims, separate blocks, or like sections to facilitate IQI positioning; radiographic location and identification markers; and radiographic density measurement device. The test method shall meet the radiographic coverage, radiographic film quality, radiographic quality level, acceptance level, and radiographic density limitations. Procedures for surface preparation, radiation application and protection, IQI selection and placement, shim utilization, radiograph identification, and single-wall or double-wall radiographic techniques are addressed.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This test method provides a uniform procedure for radiographic examination of weldments using industrial radiographic film. Requirements expressed in this method are intended to control the quality of the radiographic images and are not intended for controlling acceptability or quality of welds.
1.2 The radiographic extent, the quality level, and the acceptance criteria to be applied shall be specified in the contract, purchase order, product specification, or drawings.
1.3 The radiographic techniques stated herein provide adequate assurance for defect detectability; however, it is recognized that, for special applications, specific techniques using more or less stringent requirements may be required than those specified. In these cases, the use of alternative radiographic techniques shall be as agreed upon between purchaser and supplier (also see Section 4).
1.4 The values stated in inch-pound units are to be regarded as standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. (For more specific safety precautionary information, see Section 7.)
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
Other StandardsISO5579 Nondestructive TestingRadiographic Examination of Metallic Materials by X and Gamma RaysBasic Rules
E94 Guide for Radiographic Examination
E242 Reference Radiographs for Appearances of Radiographic Images as Certain Parameters are Changed
E390 Reference Radiographs for Steel Fusion Welds
E543 Specification for Agencies Performing Nondestructive Testing
E747 Practice for Design, Manufacture and Material Grouping Classification of Wire Image Quality Indicators (IQI) Used for Radiology
E999 Guide for Controlling the Quality of Industrial Radiographic Film Processing
E1025 Practice for Design, Manufacture, and Material Grouping Classification of Hole-Type Image Quality Indicators (IQI) Used for Radiology
E1079 Practice for Calibration of Transmission Densitometers
E1254 Guide for Storage of Radiographs and Unexposed Industrial Radiographic Films
E1316 Terminology for Nondestructive Examinations
E1815 Test Method for Classification of Film Systems for Industrial Radiography
ASNT StandardsANSI/ASNT-CP-189 Standard for Qualification and Certification of Nondestructive Testing Personnel
ICS Number Code 25.160.40 (Welding joints and welds)
UNSPSC Code 73121614(Non destructive testing service)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E1032-12, Standard Test Method for Radiographic Examination of Weldments, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top